| ||Format||Pages||Price|| |
|4||$37.00||  ADD TO CART|
|Hardcopy (shipping and handling)||4||$37.00||  ADD TO CART|
|Standard + Redline PDF Bundle||8||$44.40||  ADD TO CART|
This specification covers the standard requirements for porous nonreinforced concrete pipe for use in underdrains. The pipe shall be of two classes, identified as: “standard-strength porous nonreinforced concrete pipe” and “extra-strength porous nonreinforced concrete pipe.” The concrete shall consist of cementitious materials and water; wherein, the cement shall conform to the requirements for Portland cement or shall be Portland blast-furnace slag cement, slag-modified Portland cement, or Portland-pozzolan cement. The fly ash and ground granulated blast furnace slag shall conform to the requirements of Class F or C and Grade 100 or 120, respectively while the synthetic fibers shall be made of collated fibrillated virgin polypropylene fibers. Design requirements shall be in accordance with the internal designated diameter, wall thickness, laying length, socket depth, three-edge bearing strength, and infiltration or porosity. The pipe shall be subjected to steam curing, water curing, or combination of the two methods for a sufficient length of time to develop the specified strength requirement. Crushing tests shall be performed to determine the crushing strength of the pipes.The concrete shall consist of cementitious materials, mineral, aggregates, and water. The joints shall be of such design and the ends of the concrete pipe sections so formed that the pipe can be laid together to make a continuous line pipe. The aggregates shall be sized, graded, proportioned, and mixed with such proportions of cementitious materials, and water as will produce a homogeneous concrete mixture of such quality that the pipe will conform to test and design requirements. Pipe shall be subjected to curing. Special shapes or fittings for use with concrete pipe conforming to this specification shall be made of porous or nonporous concrete in such manner as will provide strength at least equal to the class of the adjacent pipe to which they are joined; and shall conform to all other requirements specified for pipe. The test pipe shall freed from all visible moisture. When dry, each pipe shall be measured and inspected. The crushing strength of the porous material as well as its infiltration, shall conform to the requirements.
This abstract is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.
Significance and Use
1.1 This specification covers porous nonreinforced concrete pipe for use in underdrains.
1.2 A complete metric companion to this specification has been developed
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
C33 Specification for Concrete Aggregates
C150 Specification for Portland Cement
C497 Test Methods for Concrete Pipe, Manhole Sections, or Tile
C595 Specification for Blended Hydraulic Cements
C618 Specification for Coal Fly Ash and Raw or Calcined Natural Pozzolan for Use in Concrete
C822 Terminology Relating to Concrete Pipe and Related Products
C989 Specification for Slag Cement for Use in Concrete and Mortars
C1116 Specification for Fiber-Reinforced Concrete and Shotcrete
UNSPSC Code 40171510(Commercial concrete pipe)